2 Contents Introduction 2 Rigid pavement performance 2 Pavement conditions and defects 3 Evaluation 4 Surface defects 4 Joints 7 Pavement cracks 9 Pavement deformation 12 Rating pavement surface condition 15 Rating system 16 Rating 10 & 9 Excellent 17 Rating 8 Very Good 18 Rating 7 Good 19 Rating 6 Good 20 Rating 5 Fair 21 Rating 4 Fair 23 Rating 3 Poor 24 Rating 2 Very Poor 25 Rating 1 Failed 26 Practical advice on rating roads 27 This manual is intended to assist local officials in understanding and rating the surface condition of concrete pavements. It describes types and causes of distress and provides a simple system to visually rate pavement condition. The rating procedure can be used as condition data for the Wisconsin DOT local road inventory and as part of a computerized pavement management system like PASERWARE. Produced by the T.I.C. with support from the Federal Highway Administration, the Wisconsin Department of Transportation, and the University of Wisconsin-Extension. The T.I.C., part of the nationwide Local Technical Assistance Program (LTAP), is a Center of the College of Engineering, Department of Engineering Professional Development, University of Wisconsin-Madison. Copyright 1989, 2002 Wisconsin Transportation Information Center 432 North Lake Street Madison, WI phone 800/ fax 608/ URL Printed on recycled paper.
3 Pavement Surface Evaluation and Rating PASER Manual Concrete Roads Donald Walker, T.I.C. Director, author Lynn Entine, Entine & Associates, editor Susan Kummer, Artifax, designer
4 Pavement Surface Evaluation and Rating Concrete PASER Manual Many local agencies are responsible for maintaining roadways with concrete pavements. This manual offers useful information for planning maintenance and managing Portland Cement Concrete pavements. It discusses common problems and typical repairs and includes a visual system for evaluating and rating concrete pavements. The Wisconsin Transportation Information Center has developed PASER manuals for other pavement types (see page 29). The rating systems are similar and compatible so that local road agencies can work with a comprehensive condition rating method. The rating procedure can be used as condition data for the Wisconsin DOT local road inventory (WISLR) and as part of a computerized pavement management system like PASERWARE. Taking an organized approach to roadway management has many benefits. By documenting the actual conditions of roads you can set realistic budgets, make timely repairs, and set up cost effective maintenance procedures. Developing an overall plan for the roadway system lets local agencies develop budgets and plan for future needs. When detailed information is available, local officials can respond more effectively to questions from the public. A planned approach is easier to explain and receives greater public support. Several key steps are necessary to develop a meaningful roadway management plan. First, you must inventory the existing condition. This is normally done by dividing the roadway into segments with similar conditions. During the inventory you collect information on construction history, roadway width, etc. Then you need some method for assessing the condition of the existing roadway. This Concrete PASER Manual uses a visual approach. Other information from material sampling, testing, and traffic counts can be useful when planning specific projects. Another necessary step is setting priorities for roadway improvements. You can use roadway condition and the local importance of these roads to assign priorities. Then budgets can be developed based on cost estimates for the projected improvements. Since not all improvements can be made in one year, you can set up a 3-5 year budget and capital improvement plan. Normally this is updated annually. Rigid pavement performance Most concrete pavements on local roads are either plain (non-reinforced) or reinforced concrete. Reinforcement is usually provided by steel wire mesh placed approximately at mid slab depth. The reinforcement is intended to limit crack opening and movement in the concrete slab. Since concrete slabs need to move (expand and contract) while curing and as temperature changes, pavements are constructed with contraction joints to control cracking. These are usually sawn into the pavement shortly after initial curing. This joint gives the slab a place to crack and makes a straight, well-formed groove to seal. Expansion joints are occasionally provided. These are wider, full depth, and filled with a material to allow expansion. If used, they are placed adjacent to structures that cannot move with the pavement such as bridges, manholes, and other utility structures.
5 PASER Evaluation 3 So-called rigid pavements (concrete) carry traffic loadings differently than flexible pavements (asphalt). Concrete pavements are designed to act like a beam and use the bending strength of the slabs to carry the load. Therefore load transfer across cracks and joints is important, especially on roads with heavy truck and bus traffic. Hairline and narrow cracks still have interlocked concrete aggregate and can effectively transfer loads. Because wide cracks and widely-spaced joints open up, they cannot transfer loads and must take higher edge loads. These higher edge loads can cause further cracking and deterioration along the joint or crack edges. Some concrete pavements use joints that have load transfer dowels. These are smooth steel bars placed across the joint. They transfer traffic loads between adjacent concrete slabs while allowing opening and closing of the joint. These bars can rust and sometimes cause problems. The corrosion causes forces on the concrete which lead to spalling, cracking and general joint deterioration. Epoxy coated dowels are now commonly used. Unsupported slab edges will deflect or bend under a load. If the supporting soil is saturated it can squirt up through joints or cracks when the slab bends. This is called pumping. Eventually the loss of supporting soil through pumping creates an empty space or void under the slab. The slabs may then crack further under loads and joints deteriorate more. Undoweled joints under heavy truck traffic may fault. This is when one slab edge is lower than the next slab. The downstream traffic slab will be lower than the upstream slab, creating a step. Faulting creates a poor ride. You can often detect pumping by the soil stains around pavement joints or cracks. The resulting voids can be filled with grout. Slabs can be leveled by slab jacking or mud jacking. Obviously, sealing cracks and joints and improving drainage of the subsoils will help reduce pumping, faulting, and joint failures. Pavement conditions and defects It is helpful to separate various conditions common to concrete pavements. These are described individually in some detail. We also include causes for deterioration and common strategies for repair. Some defects are localized while others indicate that problems may develop throughout the pavement. It is important to distinguish between local and widespread defects. Assessing the conditions of actual roadways also involves looking for combinations of these individual defects. Surface defects Wear and polishing, map cracking, pop-outs, scaling, shallow reinforcing, spalling. Joints Longitudinal joint, transverse joints. Pavement cracks Transverse slab cracks, D-cracking, corner cracks, meander cracks. Pavement deformation Blow ups; faulting; pavement settlement or heave; utility repairs, patches and potholes; manhole and inlet cracking; curb or shoulder deformation. In reviewing the different defects it is important to consider both their severity and extent. Generally, conditions begin slowly and progressively become more serious. Slight defects may grow into moderate and then severe conditions. In addition, the defects might initially be indicated only in a few isolated cases. Examples in the rating section will help you identify how bad a condition is and how extensive it is.
6 4 EVALUATION Surface Defects SURFACE DEFECTS Wear and polishing A worn or polished surface may appear from traffic wearing off the surface mortar and skid resistant texture. Extensive wear may cause slight ruts where water can collect and cause hydroplaning. Sometimes traffic may polish aggregates smooth, causing the surface to be slippery. An asphalt overlay or grinding of the concrete surface can restore skid resistance and remove ruts. Surface mortar worn away exposing larger aggregate. Accidents or friction testing may indicate a slippery surface in need of improved texture. Map cracking A pattern of fine cracks usually spaced within several inches is called map cracking. It usually develops into square or other geometrical patterns. Can be caused by improper cure or overworking the surface during finishing. If severe, cracks may spall or surface may scale. Repair is usually limited to very severe conditions. An asphalt overlay or partial depth patching may then be necessary. Pop-outs Individual pieces of large aggregate may pop out of the surface. This is often caused by chert or other absorbent aggregates that deteriorate under freeze-thaw conditions. Surface patching can be done temporarily with asphalt. For severe areas, a more permanent partial depth concrete patch may be necessary. Close-up of a polished pavement surface. Hairline surface cracks, probably shallow in depth. May not cause any long term performance problems. Extensive popouts of large aggregate from surface. Popouts alone have not affected pavement serviceability.
7 EVALUATION Surface Defects 5 Moderate surface scaling. Loss of mortar and fines from the surface beginning to expose larger aggregate. Severe scaling. Some larger aggregate is loose. Reinforcing bar exposed. Shallow concrete cover caused large spall to develop around it. Scaling Scaling is surface deterioration that causes loss of fine aggregate and mortar. More extensive scaling can result in loss of large aggregate. Often caused by using concrete which has not been air-entrained, the surface becomes susceptible to freeze-thaw damage. Scaling is also aggravated by the use of deicing chemicals. Scaling can occur as a general condition over a large area or be isolated to locations where poor quality concrete or improper finishing techniques caused loss of air entrainment. In severe cases, deterioration can extend deep into the concrete. Traffic action may accelerate scaling in the wheel paths. Grinding may remove poor quality surface concrete. Asphalt overlays or a bonded concrete resurfacing can prolong the life of the pavement. Partial depth patching of isolated areas may also be used. Shallow reinforcing If the steel reinforcing bar or mesh is placed too close to the concrete surface it will lead to concrete spalling. Corrosion of the steel creates forces that break and dislodge the concrete. Often you can see rust stains in the surface cracks before spalling occurs. Can be temporarily patched with asphalt. Permanent repairs are difficult and usually involve replacing the steel and making a partial depth or full depth concrete repair. Surface stain parallel to joint. Indicates reinforcing steel too close to surface. Wire reinforcing mesh placed close to surface. Corrosion of the reinforcing steel causes the surface mortar to spall. Very difficult to patch and repair.
8 6 EVALUATION Surface Defects Spalling Spalling is the loss of a piece of the concrete pavement from the surface or along the edges of cracks and joints. Cracking or freeze-thaw action may break the concrete loose, or spalling may be caused by poor quality materials. Spalling may be limited to small pieces in isolated areas or be quite deep and extensive. Repair will depend on the cause. Small spalled areas are often patched. Spalling at joints may require full depth joint repair. Small surface spalls that have been patched. Spalling along longitudinal joints. A severely spalled crack. Spalling over shallow reinforcing.
9 EVALUATION Joints 7 JOINTS Longitudinal joints New, wellsealed longitudinal joint. Joint open about 1 2. Longitudinal paving joints are constructed to be narrow in width and usually well sealed. As pavements age and materials deteriorate, joints may open and further deteriorate. Cracks parallel to the initial joint may develop and accelerate into spalling or raveling of the longitudinal joint. Settlement, instability, or pumping of the subgrade soil can cause longitudinal joints to fault. One common cause of cracks parallel to the longitudinal joints is waiting too long after the pour to saw the joint. Then, during initial cure the slab will crack roughly parallel (but not exactly) to the sawn joint. Maintaining a tight joint seal can prevent intrusion of water and reduce freeze-thaw damage and pumping. Severe joint deterioration may require full depth patching and replacement of the joint. Additional joint cracking, spalling, and broken pavement. Full depth repair is needed. Faulted longitudinal joint (over 1 2 ) with slight edge spalling.
10 8 EVALUATION Joints Transverse joints Transverse joints are constructed in concrete pavements to permit movement of the concrete slabs. Some joints are constructed with load transfer dowels. If the pavement has poor subsurface drainage, traffic may eventually create voids under the joints due to pumping and cause the slabs to settle or fault. Freeze-thaw deterioration at the joint can cause spalling and create additional cracks parallel to the joint. Load transfer bars may corrode, creating expansive forces that further deteriorate the concrete at the joint. Occasionally, severe joint deterioration may develop from poor quality aggregate and so-called D-cracking. Joint sealing will help, but complete replacement is usually necessary. Overall, lack of joint maintenance and rehabilitation is a common problem. Maintaining a tight, well sealed joint can reduce water intrusion and thereby reduce freeze-thaw damage, pumping, blow-ups, D- cracking, and spalling. Early repair of minor defects can often reduce the need for complete joint repair or replacement. New, well-sealed transverse joint. Severe spalling of a transverse joint. Cracks parallel to joint. Dark color next to transverse joint likely indicates D-cracking and additional deterioration. Full depth repair required. Transverse joint has slight faulting and spalling. Severe spalling has required temporary patching. Complete joint replacement is necessary.
11 EVALUATION Pavement Cracks 9 PAVEMENT CRACKS Transverse slab cracks Transverse cracks may appear parallel to joints and can be caused by thermal stresses, poor subgrade support, or heavy loadings. They are sometimes related to slabs having joints spaced too widely. Joints spaced more than 15 apart commonly develop mid-slab transverse cracks. Transverse, open crack. Faulted transverse crack with slight edge spalling. As with joints, these cracks may deteriorate further if not sealed well. Slabs can fault at cracks which can spall and develop additional parallel cracking. Severe deterioration may require patching individual cracks. Multiple transverse cracks in individual slabs indicate further deterioration. Extensive transverse cracking indicates pavement failure and the need for complete replacement. Closely spaced, hairline transverse cracks. Indicates slab is broken and in need of replacement.
12 10 EVALUATION Pavement Cracks D-cracks Occasionally, severe deterioration may develop from poor quality aggregate. So called D-cracking develops when the aggregate is able to absorb moisture. This causes the aggregate to break apart under freeze-thaw action which leads to deterioration. Usually, it starts at the bottom of the slab and moves upward. Fine cracking and a dark discoloration adjacent to the joint often indicate a D-cracking problem. Once this is visible on the surface the pavement material is usually severely deteriorated and complete replacement is required. Joint or crack sealing helps slow D-cracking deterioration. This is a serious defect because it may indicate a material quality problem throughout the pavement. Surface discoloration near joints and cracks indicates D-cracking and severe slab deterioration. Multiple crack patterns adjacent to joints. Common D-cracking pattern. Corner cracks Diagonal cracks near the corner of a concrete slab may develop, forming a triangle with a longitudinal and transverse joint. Usually these cracks are within one foot of the corner of the slab. They are caused by insufficient soil support or concentrated stress due to temperature related slab movement. The corner breaks under traffic loading. They may begin as hairline cracks. Some corner cracks extend the full depth of the slab while others start at the surface and angle down toward the joint. With further deterioration, more cracking develops; eventually the entire broken area may come loose. This may be a localized failure or may point to widespread maintenance problems. Partial or full depth concrete patching or full depth joint replacement may be necessary when corner cracking is extensive. First signs of corner cracking. Corner cracking with broken concrete pieces. Severely spalled corner crack with missing pieces and patching.
13 EVALUATION Pavement Cracks 11 Meander cracks Some pavement cracks appear to wander randomly. They may cross a slab diagonally or meander like a serpent. Meander cracks may be caused by settlement due to unstable subsoil or drainage problems, or by utility trench settlement. Frost heave and spring thaw can also cause them. They are often local in nature and may not indicate general pavement problems. Minor cracks may benefit from sealing to minimize water intrusion. Extensive or severe meander cracking may require replacing the slab, stabilizing the subsurface, or improving drainage. Meander crack roughly parallel to longitudinal joint. Meander crack caused by settlement. Lack of maintenance allows water to intrude and debris to collect in crack. Faulting and spalling of a meander crack.
14 12 EVALUATION Pavement Deformation PAVEMENT DEFORMATION Blowups Concrete slabs may push up or be crushed at a transverse joint. This is caused by expansion of the concrete where incompressible materials (sand, etc.) have infiltrated into poorly sealed joints. As a result, there is no space to accommodate expansion. It is more common in older pavements with long joint spacing. Pressure relief joints can be installed and blowup areas must be patched or reconstructed. Faulting Joints and cracks may fault or develop a step between adjacent slabs. Faulting is caused by pumping of subgrade soils and creation of voids. Heavy truck or bus traffic can rapidly accelerate faulting. Longitudinal joints may fault due to settlement of an adjacent slab. Faulting creates a poor ride and may cause slab deterioration. Minor faulting can be corrected by surface grinding. Voids can be subsealed, or slabs mud jacked back to level position. Severe cases may need joint replacement. Internal pressure has partially raised slab at the joint. Complete replacement is required. A pavement blowup in progress. Concrete is crushed and slabs buckled. Faulted longitudinal joint. Minor faulting of transverse joints. Aggravated by heavy traffic. Surface grinding will improve ride. Severely faulted joint. Slab jacking is necessary.
15 EVALUATION Pavement Deformation 13 Settlement caused meander crack with faulting. Extensive cracking and patching caused by settlement. Pavement was built on unstable subgrade soils. Pavement settling or heave Unstable or poorly drained subgrade soils may cause pavements to settle after construction. Poorly compacted utility trenches may also settle. This may be a gentle swale or a fairly severe dip. Frost-susceptible soils and high water tables can cause pavements to heave during the winter months. Extensive pavement cracking and loss of strength during the spring can result in severe deterioration. Improved drainage and stabilization of subgrade soils are usually necessary, along with pavement reconstruction. Utility repairs, patches and potholes Replacement or repair of utilities will require cuts or utility openings. When repaired these pavement patches may show settlement, joint deterioration, or distress under continued traffic loading. Patches from previous repairs may perform like original pavement or experience joint deterioration or settlement. Localized failures of materials or subgrade soil can cause individual potholes. Surface spalling or other material defects may develop into localized potholes. Full depth patching is usually required. Utility repair or full depth joint repair. Very good condition. Asphalt patches. Poor (top) and fair (bottom) condition. Potholes caused by severe joint deterioration. Need repair.
16 14 EVALUATION Pavement Deformation Manhole and inlet cracks Normal pavement movement due to frost heaving and movements due to changes in temperature often cannot be accommodated in the pavement adjacent to a manhole or a storm sewer inlet. Cracks and faulting may develop and the concrete slab may deteriorate further. These are often localized defects that may not indicate a general pavement problem. Sealing and patching may slow the deterioration. Eventually full depth repairs may be required. Curb or shoulder deformation Concrete curb and gutter, or paved concrete shoulders, may separate from or settle along the main pavement. The longitudinal joints between the pavement and curb or shoulder may open, fault, or deteriorate like other longitudinal joints. When severe enough to disrupt drainage, the curb and gutter need to be replaced. Shoulder deterioration may require patching or replacement. Two spalls at manhole in a new pavement. Partial depth patching would be beneficial. Extensive cracking and spalling at manhole requiring full depth repairs. Settled gutter and joint filled with debris. Joint maintenance is needed. Extensive curb deterioration. Freeze-thaw damage to curb adjacent to inlet, and gutter is displaced. New curb and gutter are needed.
17 15 Rating pavement surface condition With an understanding of roadway conditions and distress, you can evaluate and rate concrete pavements. The rating scale ranges from 10 excellent condition to 1 failed. In general, most pavements will deteriorate through the phases listed in the rating scale. However, it is common for pavements to skip several levels when major defects appear or when the pavement is repaired. The time it takes to go from an excellent (10) to a very poor condition (1) depends largely on the quality of the original construction and the amount of heavy traffic loading. Once significant deterioration begins it is common to see pavements deteriorate rapidly. This is usually due to the combined effects of loading and additional moisture. As a pavement ages and additional cracking develops, more moisture can enter the pavement and accelerate the rate of deterioration. Look at the photographs which follow and become familiar with the descriptions of the individual rating categories. To evaluate an individual pavement segment, first determine its general condition. Is it relatively new, toward the top end of the scale? In very poor condition and at the bottom of the scale? Or somewhere in between? Next, think generally about the appropriate maintenance method. Finally, review the individual pavement condition and distress and select the appropriate pavement rating. Remember that individual pavements will not have all of the types of distress listed for any particular rating. They may have only one or two types. Use the categories in the table below and on page 16. We have found that relating a normal maintenance or rehabilitation procedure to the surface rating scheme helps you use the rating system. However, choosing an individual surface rating should not automatically dictate the final maintenance or rehabilitation technique. You should consider safety, future traffic projections, original construction, and pavement strength since these may dictate a more comprehensive rehabilitation. On the other hand, it may be appropriate under special conditions to do nothing and let the pavement fully deteriorate and then rebuild when funds are available. RATINGS ARE RELATED TO NEEDED MAINTENANCE OR REPAIR Rating 9 & 10 Rating 7 & 8 Rating 5 & 6 Rating 3 & 4 Rating 1 & 2 New pavement or recent concrete rehabilitation. No maintenance required. First signs of wear, scaling, or cracking. Needs routine maintenance. First signs of corner cracks, faulting, and joint or crack spalling. Requires surface repairs, sealing or partial depth patching. Moderate to severe faulting, multiple slab cracking, and joint failure. Requires extensive slab or joint rehabilitation. Pavement failure requiring complete reconstruction.
18 16 Rating pavement surface condition Rating system Surface rating Visible distress* General condition/ treatment measures 10 Excellent None. New pavement. No maintenance required. 9 Excellent Traffic wear in wheelpath. Slight map cracking or pop-outs. Recent concrete overlay or joint rehabilitation. Like new condition. No maintenance required. 8 Very Good Pop-outs, map cracking, or minor surface defects. Slight surface scaling. Partial loss of joint sealant. Isolated meander cracks, tight or well sealed. Isolated cracks at manholes, tight or well sealed. More surface wear or slight defects. Little or no maintenance required. 7 Good More extensive surface scaling. Some open joints. Isolated transverse or longitudinal cracks, tight or well sealed. Some manhole displacement and cracking. First utility patch, in good condition. First noticeable settlement or heave area. First sign of transverse cracks (all tight); first utility patch. More extensive surface scaling. Seal open joints and other routine maintenance. 6 Good Moderate scaling in several locations. A few isolated surface spalls. Shallow reinforcement causing cracks. Several corner cracks, tight or well sealed. Open ( 1 4 wide) longitudinal or transverse joints and more frequent transverse cracks (some open 1 4 ). First signs of shallow reinforcement or corner cracking. Needs general joint and crack sealing. Scaled areas could be overlaid. 5 Fair Moderate to severe polishing or scaling over 25% of the surface. High reinforcing steel causing surface spalling. Some joints and cracks have begun spalling. First signs of joint or crack faulting ( 1 4 ). Multiple corner cracks with broken pieces. Moderate settlement or frost heave areas. Patching showing distress. First signs of joint or crack spalling or faulting. Grind to repair surface defects. Some partial depth patching or joint repairs needed. 4 Fair Severe polishing, scaling, map cracking, or spalling over 50% of the area. Joints and cracks show moderate to severe spalling. Pumping and faulting of joints ( 1 2 ) with fair ride. Several slabs have multiple transverse or meander cracks with moderate spalling. Spalled area broken into several pieces. Corner cracks with missing pieces or patches. Pavement blowups. Needs some full depth repairs, grinding, and/or asphalt overlay to correct surface defects. 3 Poor Most joints and cracks are open, with multiple parallel cracks, severe spalling, or faulting. D-cracking is evident. Severe faulting (1 ) giving poor ride. Extensive patching in fair to poor condition. Many transverse and meander cracks, open and severely spalled. Needs extensive full depth patching plus some full slab replacement. 2 Very Poor Extensive slab cracking, severely spalled and patched. Joints failed. Patching in very poor condition. Severe and extensive settlements or frost heaves. Recycle and/or rebuild pavement. 1 Failed Restricted speed. Extensive potholes. Almost total loss of pavement integrity. Total reconstruction. * Individual pavements will not have all of the types of distress listed for any particular rating. They may have only one or two types.
19 Rating pavement surface condition 17 RATING 10 & 9 EXCELLENT No maintenance required Rating 10 is for new pavement. Rating 9 is used for recent concrete rehabilitation or likenew condition. Some traffic wear. Slight map cracking or pop-outs. No maintenance required. RATING 10 New pavement with integral curb. RATING 9 Like new condition. RATING 9 Recent joint rehabilitation. Like new condition.
20 18 Rating pavement surface condition RATING 8 VERY GOOD Little or no maintenance required More surface wear, or slight defects showing in lanes. Pop-outs, slight surface scaling, partial loss of joint sealant, or isolated meander crack. Isolated manhole distress. Little or no maintenance required. Slight scaling. Isolated spall at manhole. Partial loss of joint sealant. Isolated meander crack, tight and well sealed.
21 Rating pavement surface condition 19 RATING 7 GOOD May require some routine sealing or maintenance First signs of transverse cracking, patching or repair; more extensive pop-outs or scaling; some manhole displacement, isolated heave or settlement. May need some sealing or routine maintenance. Residential street pavement in good condition after many years of service. May only need periodic joint sealing maintenance. Extensive pop-outs. Pavement is unsightly but still provides good level of service. Recent full depth pavement repair. In very good condition. Well sealed transverse crack. Joint repairs in good condition. Transverse crack. Tight, sound pavement.
22 20 Rating pavement surface condition RATING 6 GOOD Joint and crack sealing needed First signs of corner cracking or shallow reinforcement. More frequent transverse cracks. Open ( 1 4 ) joints and cracks. Moderate scaling. Needs joint and crack sealing. Several transverse cracks. Tight or well sealed. Surface rust stain. Indicates shallow reinforcing. Moderate scaling. First signs of corner cracks. Isolated, tight meander crack. Several pop-outs. Remaining joints and cracks all tight and sound.
23 Rating pavement surface condition 21 RATING 5 FAIR Partial depth patching and joint repairs may be needed First signs of joint or crack spalling, or faulting. Multiple cracking at corners with broken pieces. Patching in fair condition. Surface texturing repairs may be necessary. Some partial depth patching and joint repairs may be needed. Faulting at longitudinal joint and spalling along joint edge. First signs of transverse joint faulting. Grinding will improve ride. Open cracks with edge spalling. Corner crack and broken corner piece. Isolated manhole problems and joint spalling. Full depth repair required adjacent to manhole.
24 22 Rating pavement surface condition RATING 5 FAIR (continued) Partial depth patching and joint repairs may be needed Patching in fair condition. Broken corner pieces. Some joint spalling. Severe scaling over extensive areas. Patching or overlay needed. Spalling caused by shallow reinforcing steel. Temporary patching needs to be followed by extensive partial depth repairs.
25 Rating pavement surface condition 23 Wide open meander crack (1 ) with edge spalling. Corner crack with spalling. RATING 4 FAIR Some full depth joint or crack repair required Severe surface distress requires asphalt overlay or extensive surface texturing. Multiple transverse cracks with spalling and broken pieces. Corner cracking with potholes or patches. Blowups. Some full depth joint or crack repair required. All joints show some deterioration and spalling. Multiple open transverse cracks. Failed corner crack. Patches in fair condition. Moderate spalling at transverse joint. Corner cracking developed into small hole; moderate spalling of transverse crack. Moderate to severe longitudinal joint faulting. Transverse joint also has spalling.
26 24 Rating pavement surface condition RATING 3 POOR Extensive full depth patching plus some full slab replacement required Multiple transverse cracks. Poor longitudinal joint with spalling. Most joints and cracks are open (1 ), spalled, or patched. D-cracking is evident. Severe (1 ) faulting. Extensive full depth patching required plus some full slab replacement. Joints and cracks badly spalled. Patching is failing. Full depth repairs required. D-cracking (discoloration) at transverse joint and corner cracking. Needs full-depth repair. Discoloration at joints indicates D-cracking. Slab replacement needed. Badly spalled joint and open crack. Slab or joint replacement needed. Failed joint needs replacement.
27 Rating pavement surface condition 25 RATING 2 VERY POOR Pavement recycling and reconstruction necessary Failed patches. Replace entire portion of lane. Remove and replace pavement around manhole and inlet. Closely spaced transverse cracks and poor longitudinal joint. Replace slab. Severe deterioration. Requires extensive reconstruction. Extensive joint failure. Major rehabilitation or complete replacement needed.
29 27 Practical advice on rating roads Inventory and field inspection Most agencies routinely observe roadway conditions as a part of their normal work and travel. However, an actual inspection means looking at the entire roadway system as a whole and preparing a written summary of conditions. This inspection has many benefits over casual observations. It can be helpful to compare segments, and ratings decisions are likely to be more consistent because the roadway system is considered as a whole within a relatively short time. An inspection also encourages a review of specific conditions important in roadway maintenance, such as drainage, adequate strength, and safety. A simple written inventory is useful in making decisions where other people are involved. You do not have to trust your memory, and you can usually answer questions in more detail. Having a written record also improves your credibility with the public. Finally, a written inventory is very useful in documenting changing roadway conditions. Without records over several years, it is impossible to know if your overall road conditions are improving, holding their own, or declining. Annual budgets and long range planning are best done when based on actual needs as documented with a written inventory. The Wisconsin DOT local road inventory (WISLR) is a valuable resource for managing your local roads. Adding PASER surface condition ratings is an important improvement. Averaging and comparing sections For evaluation, divide the local road system into individual segments which are similar in construction and condition. Rural segments may vary from 1 2 mile to a mile long, while sections in urban areas will likely be 1-4 blocks long or more. If you are starting with the WISLR Inventory, the segments have already been established. You may want to review them for consistent road conditions. Obviously no roadway segment is entirely consistent. Also, individual pavements will not have all of the types of distress listed for any particular rating. They may have only one or two types. Therefore, some averaging is necessary. The objective is to rate the condition that represents the majority of the roadway. Small or isolated conditions should not influence the rating. It is useful to note special conditions on the inventory form so this information can be used in project design. For example, some spot repairs may be required. Occasionally pavement conditions will vary significantly. For example, short sections of good condition may be followed by sections of poor pavement conditions. In this case, it is best to rate the pavement according to the worst conditions and note the variation on the form. The overall purpose of condition rating is to be able to compare each segment relative to all the other segments in your roadway system. On completion you should be able to look at any two pavement segments and find that the better surface has a higher rating. Within a given rating, say 6, not all pavements will be exactly the same. However, they should all be considered to be in better condition than those with lower ratings, say 5. Sometimes it is helpful in rating a difficult segment to compare it to other previously rated segments. For example, if it is better than one you rated 5, and worse than a typical 7, then a rating of 6 is appropriate. Having all pavement segments rated in the proper relative order is important and useful. Assessing drainage conditions Moisture and poor pavement drainage are significant factors in pavement deterioration. Some assessment of drainage conditions during pavement rating is highly recommended. While you should review drainage in detail at the project level, at this stage simply include an Urban drainage. RATING: Excellent Adequate rural ditch and good erosion control. RATING: Good
30 28 Practical advice on rating roads overview drainage evaluation at the same time as you evaluate surface condition. Look at the roadway crown and check for low surface areas that permit ponding. Paved surfaces should have approximately a 2% cross slope or crown across the roadway. Rural Reshape terrace behind curb to restore drainage and prevent damage to curb and street. RATING: Fair shoulders should have a greater slope to improve surface drainage. Good drainage improves a pavement s ability to resist pumping, faulting and joint damage. Some new concrete pavements are being constructed with a special drainage layer and drain system to reduce water-related deterioration. These systems require inspection and periodic maintenance. You should also check curb and gutter, culverts, and storm drain systems. Storm drainage systems that are silted in, have a large accumulation of debris, or are in poor structural condition will also degrade pavement performance. The T.I.C. publication, Drainage Manual: Local Road Assessment and Improvement, describes the elements of drainage systems, depicts them in detailed photographs, and explains how to rate their condition. Copies are available from the T.I.C. Planning annual maintenance and repair budgets We have found that relating a normal maintenance or rehabilitation procedure to the surface rating scheme helps local officials use the rating system. However, an individual surface rating should not automatically dictate the final maintenance or rehabilitation technique. You should consider safety, future traffic projections, original construction, and pavement strength since these may dictate a more comprehensive rehabilitation than the rating suggests. On the other hand, it may be appropriate under special conditions to do nothing and let the pavement fully deteriorate, then rebuild when funds are available. Summary Using local road funds most efficiently requires good planning and accurate identification of appropriate rehabilitation projects. Assessing roadway conditions is an essential first step in this process. This concrete pavement surface condition rating procedure has proved effective in improving decision making and using roadway funds more efficiently. It can be used directly by local officials and staff. It may be combined with additional testing and data collection in a more comprehensive pavement management system. Flooding. Curb and gutter need reconstruction. RATING: Poor
31 Transportation Information Center Publications Pavement Surface Evaluation and Rating (PASER) Manuals Asphalt PASER Manual, 2002, 28 pp. Brick and Block PASER Manual, 2001, 8 pp. Concrete PASER Manual, 2002, 28 pp. Gravel PASER Manual, 2002, 20 pp. Sealcoat PASER Manual, 2000, 16 pp. Unimproved Roads PASER Manual, 2001, 12 pp. Drainage Manual Local Road Assessment and Improvement, 2000, 16 pp. SAFER Manual Safety Evaluation for Roadways, 1996, 40 pp. Flagger s Handbook (pocket-sized guide), 1998, 22 pp. Work Zone Safety, Guidelines for Construction, Maintenance, and Utility Operations, (pocket-sized guide), 2002, 58 pp. Wisconsin Transportation Bulletins #1 Understanding and Using Asphalt #2 How Vehicle Loads Affect Pavement Performance #3 LCC Life Cycle Cost Analysis #4 Road Drainage #5 Gravel Roads #6 Using Salt and Sand for Winter Road Maintenance #7 Signing for Local Roads #8 Using Weight Limits to Protect Local Roads #9 Pavement Markings #10 Seal Coating and Other Asphalt Surface Treatments #11 Compaction Improves Pavement Performance #12 Roadway Safety and Guardrail #13 Dust Control on Unpaved Roads #14 Mailbox Safety #15 Culverts-Proper Use and Installation #16 Geotextiles in Road Construction/Maintenance and Erosion Control #17 Managing Utility Cuts #18 Roadway Management and Tort Liability in Wisconsin #19 The Basics of a Good Road #20 Using Recovered Materials in Highway Construction #21 Setting Speed Limits on Local Roads 432 North Lake Street Madison, WI phone 800/ fax 608/ URL
Local Road Assessment and Improvement Drainage Manual Donald Walker, T.I.C. Director, author Lynn Entine, Entine & Associates, editor Susan Kummer, Artifax, design Transportation Information Center University
September 1, 2003 CONCRETE MANUAL 5-694.900 5-694.901 GENERAL CONCRETE PAVEMENT REHABILITATION 5-694.900 Concrete Pavement Rehabilitation is an extremely valuable tool of the Minnesota Department of Transportation
Page 1 Revised 3/2/10 See the DESIGN GUIDELINES in Section I-06 for requirements for cross slope of the roadway. For New/Reconstruction projects: The cross slope of the driving lanes range from 1.5% to
APPENDIX B GUIDELINES FOR IDENTIFYING AND REPAIRING LOCALIZED AREAS OF DISTRESS IN AC PAVEMENTS PRIOR TO CAPITAL PREVENTIVE MAINTENANCE OR REHABILITATION REPAIRS I. Background Information A. AC Pavement
DISTRESS IDENTIFICATION MANUAL for the Long-Term Pavement Performance Program PUBLICATION NO. FHWA-RD-03-031 JUNE 2003 In 1987, the Strategic Highway Research Program began the largest and most comprehensive
Metropolitan Builders Association Masonry & Concrete Standard Background Masonry and concrete work in residential construction often provides the base structure upon which the house is built or as a veneer.
Asphalt Maintenance Why Maintain Your Asphalt? Asphalt pavement is basically sand, gravel and glue. The glue used to keep the sand and gravel together is asphalt, a heavy by-product of oil refining. While
CONCRETE REPAIR GUIDELINES Concrete repairs can be broken down into four basic types, plus special repairs and planing. Note: It is recommended that investigation into soundness of pavement be performed
1 Most basements show some signs of leaking and cracking. Through the years, problems with water, poor soils, grading, drainage and possible settling affect the integrity of a basement. Being able to recognize
University of Pittsburgh Rehabilitation Strategies for Bonded Concrete Overlays of Asphalt Pavements Authors: J. M Vandenbossche S. Sachs August 2013 1. Introduction Bonded concrete overlays of asphalt
Long Life Concrete Pavement Joint Performance Joint Rehabilitation Gary Fick, Trinity Construction Management Services, Inc. Representing the National CP Tech Center Driving Forces for Concrete Pavement
Pavement Patching Repair for AC and PCC Pavement Surfaces Vern Thompson www.crafco.com Overview and Objective New Methods For Pavement Patching-Overview What are they How they are applied New Methods Secti
MAINTAINING HOUSTON S STREETS REPAIR, REHABILITATION, RECONSTRUCTION Using the Full Range of Tools for a Challenging Job Report To: TTI Committee May 13, 2014 1 Pavement Management - Suggested Treatments
I-66 Pavement Rehabilitation Fall Asphalt Conference Richmond, VA David Shiells, P.E. Virginia Department of Transportation David White Superior Paving Corporation October 2, 2012 Project Location 2 Goal
Sanitary Sewer Overflow (SSO) Control and Wastewater Facilities Program Sewer Rehabilitation Design Requirements City of Baton Rouge/Parish of East Baton Rouge Department of Public Works Submitted by Prepared
Transportation Asset Management Program 2009 Federal Aid PASER Road Survey August 2009 WEST MICHIGAN SHORELINE REGIONAL DEVELOPMENT COMMISSION (WMSRDC) The WMSRDC is a regional council of governments representing
Municipal Pavement Design with StreetPave Software March 5, 2009 Scott Haislip Senior VP Pavement Engineering Presentation Overview Background / history of the design procedure Concrete pavement design
Página 1 de 12 AASHO Road Test The AASHO Road Test, a $27 million (1960 dollars) investment and the largest road experiment of its time, was conceived and sponsored by the American Association of State
ABSTRACT An evaluation of the street infrastructure in Foxberry Estates Phase 1, including pavement condition, verification of construction techniques, and subgrade quality. Recommendations and costs for
Guide Specification: Diamond Grinding for City Streets Publication Date: May 24, 2010 SCOPE City streets are defined as roadways with a closed drainage system along with numerous structures such as manholes,
CALIFORNIA DEPARTMENT OF TRANSPORTATION DIVISION OF DESIGN Office of Pavement Design Pavement Design & Analysis Branch Jointed Plain Concrete Pavement (JPCP) Preservation and Rehabilitation Design Guide
CAPITAL PREVENTIVE MAINTENANCE 2003 EDITION April 8, 2010 CONSTRUCTION AND TECHNOLOGY DIVISION Attention Manual Holders This manual is to remain with the assigned user. If the user relocates within the
Safe & Sound Bridge Terminology Abutment A retaining wall supporting the ends of a bridge, and, in general, retaining or supporting the approach embankment. Approach The part of the bridge that carries
CITY AND COUNTY OF DENVER ENGINEERING DIVISION Wastewater Capital Projects Management Standard Construction Specification 10.1 Precast Concrete Pipe 10.1.1 General This section covers material requirements,
HIGHWAY DESIGN MANUAL 600-1 May 7, 2012 CHAPTERS 600 670 PAVEMENT ENGINEERING CHAPTER 600 GENERAL ASPECTS Topic 601 - Introduction Pavement engineering involves the determination of the type and thickness
Performance of Edge Drains in Concrete Pavements in California Biplab B. Bhattacharya, 1 Michael P. Zola, 2 Shreenath Rao, 3 Karl Smith, 4 Craig Hannenian 5 ABSTRACT The California Department of Transportation
Concrete Pavement Rehabilitation Rehabilitating Concrete Pavements using CPR 3 Restoration Resurfacing Reconstruction By Tim Smith Director Transportation & Public Works Cement Association of Canada, April
Session 7: Retrofitted Edge Drains 7.1 Learning Outcomes 1. List benefits of drainage 2. List components of edge drain systems 3. Describe recommended installation procedures 4. Identify typical construction
40 Sidewalk Materials Materials and Sidewalk Zones Permeable Pavement Accessibility The key components of sidewalk construction are material selection and installation. These two aspects should come together
F I N A L Construction Specifications for Keyhole Pavement Coring and Reinstatement Gas Technology Institute 1700 S. Mount Prospect Rd. Des Plaines, Illinois 60018 www.gastechnology.org Version 13 October
Guidelines for Durable Driveways, Carports Patios, Walks, Garage Floors The Right Concrete Mix Placing and Finishing Joints Correctly Spaced Curing for Durability "Concrete durability is the ability to
State of Illinois Department Of Transportation CONSTRUCTION INSPECTOR S CHECKLIST FOR STORM SEWERS While its use is not required, this checklist has been prepared to provide the field inspector a summary
Cracks, chips and broken or flaking areas in concrete are not only unsightly, they can lead to further deterioration of the surface. The result is a costly replacement project as opposed to a simple repair.
Chapter 4 Bases 4-02 Gravel Base GEN 4-02.1 General Instructions Gravel Base is typically used in the construction of the roadway section and provides support for the pavement. For the pavement to provide
Porous Pavement Alternatives Cost Analysis Prepared by Century West Engineering for Metro This cost analysis compares the construction costs of six different types of pavement for three different scenarios.
Storm Drain Inlet Protection for Construction Sites (1060) Wisconsin Department of Natural Resources Conservation Practice Standard I. Definition A temporary device installed in or around a storm drain
5 Chapter Restoration of Damaged Structures Bringing back a damaged structure to its pre-earthquake state and original strength is called restoration. This is the first step of building rehabilitation.
SECTION 014500 QUALITY CONTROL PART 1 GENERAL 1.01 RELATED REQUIREMENTS A. Drawings and General Provisions of Contract, including General and Special Conditions and other Division 1 Specification Sections,
Pavement Maintenance M A N U A L Mike Johanns Governor John Craig Director Pavement Maintenance Manual Acknowledgements........................................................................ii Introduction..............................................................................1
APPENDIX K PIPE INSPECTION **Virginia Test Method 123** Post Installation Inspection of Buried Storm Drain Pipe and Pipe Culverts June 25, 2010 SCOPE For all roadway projects that are constructed by private
Failing Culverts Structural Problems & Economic Considerations Al Tenbusch, President, Tenbusch, Inc. Brian Dorwart, Senior Associate, Brierley Associates Albert F. Tenbusch, Engineer, Tenbusch, Inc. June
Unit Price Averages Reports 12/7/2015 UNIT PRICE AVERAGES REPORT Disclaimer The information provided in the following Unit Price Averages Report is only for the use of Alberta Infrastructure & Transportation
SPECIFICATIONS FOR SEWER PIPE AND LINING INSERTION - TRENCHLESS; GENERAL GUIDELINES (As Provided by NASSCO) 1 Intent: The intent of trenchless sewer pipe Insertion is to rehabilitate the existing sewer
Pavement Rehabilitation Using Hot Mix Asphalt - National Perspective - Rehabilitation Process Evaluate Existing Pavement and Conditions Evaluate Options Construct Project Monitor Performance Evaluate Existing
Categories EC Erosion Control SE Sediment Control TC Tracking Control WE Wind Erosion Control Non-Stormwater NS Management Control Waste Management and WM Materials Pollution Control Legend: Primary Category
SD95-16-G2 SD Department of Transportation Office of Research Rural Road Design, Maintenance, and Rehabilitation Guide Prepared by ERES Consultants, Inc. 505 West University Champaign, IL 61820-3915 September
Foundations 65 5 FOUNDATIONS by Richard Chylinski, FAIA and Timothy P. McCormick, P.E. 66 Foundations Foundations 67 FOUNDATIONS Let's assume that the retrofit has been done correctly from the roofline
Appendix A Pavement Distress Types and Causes This Appendix provides descriptions of the types and causes of the distresses that occur in asphalt, concrete, and asphalt-overlaid concrete pavements, and
Concrete - Types of Concrete o QUIKRETE 5000 is the ideal choice for applications requiring high early strength. Because it gains strength quickly, it is ideal for cold weather applications. QUIKRETE 5000
How to Identify, Evaluate & Repair Shrinkage Cracks in Poured Concrete What is concrete shrinkage cracking, how and where does it occur? Are concrete floor cracks a structural problem? How to recognize
Installation PowerPoint for Grasscrete Formers 1 This document describes the two single-use tools utilized to create the Grasscrete product. The original Former is a vacuum formed light gauge plastic mold
TNZ B/02:2005 SPECIFICATION FOR CONSTRUCTION OF UNBOUND 1. SCOPE This specification shall apply to the construction of unbound granular pavement layers. The term pavement layer shall apply to any layer
Report of Turnover Survey VILLAS OF TRADITIONS AT GREY OAKS Grey Oaks Development Naples, Collier County, Florida Forge Engineering Project Number 2907-001.01 March 2015 Richard P..Lundberg, P.E cn=richard
STORM DRAIN INLET PROTECTION SE-10 Objectives Erosion Control - EC Sediment Control - SE Tracking Control - TC Wind Erosion Control - WE Non-Storm Water Management - NS Waste and Materials Management -
SPECIAL NOTE FOR ASPHALT WATERPROOFING MIX FOR BRIDGE-DECK OVERLAYS AND ADJACENT APPROACHES 1. DESCRIPTION. Asphalt Waterproofing Mix (AWM) is a highly elastomeric, polymermodified, impermeable asphalt
Objectives EC Erosion Control SE Sediment Control TR Tracking Control WE Wind Erosion Control Non-Stormwater NS Management Control Waste Management and WM Materials Pollution Control Legend: Primary Objective
1. Foundation/Basement 17 PERFORMANCE GUIDELINES 1. FOUNDATION/BASEMENT 1.1 Efflorescence on concrete or masonry surfaces Efflorescence is the formation of a white crystalline or powdery deposit on the
6 Index inlet protection excavated drop inlet protection (Temporary) 6.50.1 HARDWARE CLOTH AND GRAVEL INLET PROTECTION Block and gravel inlet Protection (Temporary) sod drop inlet protection ROCK DOUGHNUT
The contractor shall moist-cure the completed Lime Treated Subbase for a minimum of days before allowing any traffic on the compacted surface. The contractor shall be responsible for repairing any damages
Township of Enniskillen Asset Management Plan 2014 1 TABLE OF CONTENTS Page A. Introduction 3 B. State of Local Infrastructure 4 C. Desired Levels of Service 7 D. Asset Management Strategy 8 E. Financing
HIGHWAYS DEPARTMENT GUIDANCE NOTES ON THE USE OF WATERPROOFING MEMBRANES ON CONCRETE BRIDGE DECKS Research & Development Division RD/GN/033 June 2008 THE USE OF WATERPROOFING MEMBRANES ON CONCRETE BRIDGE
402.02 Section 402. STORM SEWERS 402.01. Description. This work consists of constructing storm sewers of the size and class required, including excavation, bedding, and backfill. 402.02. Materials. Provide
DESCRIPTION OF STORMWATER STRUCTURAL CONTROLS IN MS4 PERMITS Phase I MS4 permits require continuous updating of the stormwater system inventory owned and operated by the MS4. They also include inspection
CONSTRUCTION PERMIT REQUIREMENTS Any work to be done in the City right-of-way (ROW), in a utility easement, and certain work on private property, requires an Engineering Inspection Permit from the Department
APPLICATION FOR DEMOLITION & RIGHT-OF OF-WAY PERMIT City of Swartz Creek 8083 Civic Drive Swartz Creek, MI 48473 810-635-4464 Fee Received: $ Date: / / Receipt No: Demolition Permit (including Right of
02530-1 of 5 SECTION 02530 STORM DRAINAGE STRUCTURES 02530.01 GENERAL A. Description Storm drainage structure construction shall include, but not necessarily be limited to, furnishing and installing or
Fly Ash Slurry Injection (FASI) of Bituminous Thermal Cracks Schedule What is Fly Ash Slurry Injection (FASI) Thermal Cracks and Why They Depress Pavement Rehab Strategies Special Provisions Upcoming Projects
GUIDE TO BASIC FLOOR REPAIRS Basic Repair Guidelines for Common Floor Defects Including RANDOM CRACKS, SPALLED JOINTS, GOUGES, JOINT FILLER SEPARATION AND MORE... 14 CRITICAL STEPS TOWARDS ACHIEVING PERMANENT,
SECTION 55 PIPE FOR STORM DRAINS AND CULVERTS (FAA D-701) 55-1 GENERAL The Contractor shall perform all work required by the plans for construction of pipe for storm drains, precast polymer trench drains
SECTION 08000 STORM DRAINAGE 08010 DESIGN A. Location B. Sizing TABLE OF CONTENTS 08020 MATERIALS A. Pipe Materials B. Structure Materials C. Installation D. Inlets and Outlets 08030 INSPECTIONS AND TESTING
Ohio Department of Transportation Division of Production Management Office of Geotechnical Engineering Geotechnical Bulletin GB 1 PLAN SUBGRADES Geotechnical Bulletin GB1 was jointly developed by the Offices
PART 1 - GENERAL Section 02702 SEWER PIPE INSTALLATION AND TESTING 1-1. SCOPE. This section covers the installation and testing of all sewer pipe furnished under the following specification sections: Concrete
Advancements in GPR for a Sustainable Tomorrow Shawn Lapain, BSc. E., EIT Pavement Specialist Applied Research Associates Inc. 5401 Eglinton Avenue West, Suite 105, Toronto, ON, Canada, M9C 5K6 Tel: 416-621-9555,
Storm Drain Inlet Protection for Construction Sites (1060) Wisconsin Department of Natural Resources Conservation Practice Standard I. Definition A temporary device installed in or around a storm drain
Overview: 1971 N 1966 GYM 1966 CLASSROOM WING 1966 AUD. 1971 GYM 1998 1998 POOL EAST LYME HIGH SCHOOL Original 1966 Building: The original East Lyme High School was constructed in 1966 and was composed
NCMA TEK National Concrete Masonry Association an information series from the national authority on concrete masonry technology CONCRETE MASONRY FOUNDATION WALL DETAILS TEK 5-3A Details (2003) Keywords:
Shift from new construction to renewal and preservation Functional improvements for safety and smoothness needed more than structural improvements Perpetual Pavements Material improvements Binders Superpave
To Pave or Not to Pave? Making Informed Decisions on When to Upgrade a Gravel Road How to decide when to pave or not? Two new reports offer some help: Cost Comparison of Treatments Used to Maintain and
TECHNICAL NOTE Culvert Sliplining and Lining of Casings with HPPipe TN 5.14 February 2010 Introduction It may be at times necessary, in an aging infrastructure, to rehabilitate drainage and sanitary lines
Engineering & Construction Services Division Standard Specifications for Road Works TS 3.50 April 2015 for Concrete Curb and Table of Contents TS 3.50.01 SCOPE... 3 TS 3.50.02 REFERENCES... 3 TS 3.50.03
USE OF A DIGITAL SURVEY VEHICLE FOR PAVEMENT CONDITION SURVEYS AT AIRPORTS Paul W. Wilke, P.E. Applied Research Associates, Inc. August 11, 2014 Words: 3,280 Figures: 3 Tables: 0 Photographs: 3 ABSTRACT